926 Cossiello et al. Macromolecules, Vol. 38, No. 3, 2005
polymeric material cannot be discussed independently of 1-30 kHz, making it possible to distinguish rigid from
of a knowledge of their relaxation processes. mobile segments. Because the experiment is performed
It is widely recognized that the light-emitting perfor- under magic-angle spinning (MAS), this is achieved for
mances of optoelectronic devices are strongly affected each chemical group along the polymer chain in a high-
by thermally induced morphological variations, brought resolution 13C CP/MAS spectrum. More specifically, the
about by field/current Joule effects, in particular. These application of the 1D-DIPSHIFT pulse sequence31 pro-
effects are extremely deleterious to the light emission duces an echo at twice the sample rotation period, 2tr,
efficiency and durability of the devices. Thus, it is whose amplitudes are modulated by 〈cos(ωdipt1)〉, where
remarkable that the thermally induced effects in light- ωdip ) δdip(3 cos2 θ - 1)/2, δCH is the anisotropy
emitting polymers, such as MEH-PPV, have not been parameter for the heteronuclear dipolar interaction, θ
explored. To our best knowledge, only the thermal is the angle between the CH bond and the static
induced rheological transitions (the glass transition) of B
magnetic field B0, and the evolution period t130 is the
PPV thin films have been studied by shear-modulated time in which the carbon magnetization evolves under
scanning force microscopy and correlated with emissive the CH dipolar coupling, ωdip ) 2πυdip. Therefore, by
properties.19 Although the relaxation processes of MEH- measuring the signal amplitude as a function of t1,
PPV have not been reported, the importance of chain typical curves whose shape depends on υdip are obtained,
mobility has been observed in several studies, without allowing estimating this parameter. If molecular mo-
any explanation. For example, some peculiar behavior tions occurring with rates higher than 1 kHz are
around 200-220 K was noticed for spectral line nar- present, the strength of the anisotropic dipolar coupling
rowing and for the temperature dependence of the is partially or totally averaged, and as a result, motional
absorption and the photoluminescence bands of the averaged anisotropic dipolar CH coupling 〈ωdip〉 ) 2π-
polymer.17 A strong slope change of the electron injection 〈υdip〉 is measured in DIPSHIFT experiments.
barrier and for the absorption peak was observed below Experimental Section
220 K.22 The quantum efficiencies of diode-based MEH-
Materials. MEH-PPV was purchased from Aldrich, with
PPV increased with a decrease in the temperature, a molecular weight of 86 kg mol-1, according to the supplier.
which was later explained as due to the improvement It was used as received. Toluene was supplied from Merck
of the charge balance.20,21 The temperature dependences 99.5% of purity and chloroform was from Vetec, Brazil (99.8%).
of both the absorption and the photoluminescence The solvents were dried using molecular sieves (4 Å). Fresh
spectra of PPV and MEH-PPV films have shown a red solutions were used for each film preparation.
shift of the peak position upon cooling.23-27 Differences Films were spin-coated at 3000 rpm during 30 s in a
in the magnitude of the shift of absorption and photo- Headway Research Inc. model PWM32 spinner. A thickness
luminescence are on the order of kT (thermal energy) of 800 nm was determined by inspecting the film fracture
and were attributed to conformational changes of the surfaces with a JEOL JSM-6360LV scanning electron micro-
scope. The surface was sputtered with gold/palladium (80/20)
polymer chains. Freezing increases the planarity of the alloy in a Bal-Tec MED 020 MCS 010 casting system. Images
conjugated emitting center and the effective length of were recorded with an accelerating voltage of 10 kV.
the electron delocalization, producing a red shift of the Methods. Steady-state fluorescence spectroscopy was per-
emission spectrum.28 Thus, although the specific deter- formed using a system described elsewhere.33 Samples were
mination of MEH-PPV relaxation processes has not yet excited by a high-pressure mercury lamp arc (200 W) whose
been reported, the importance of these processes has excitation wavelength of 21 280 cm-1 was selected by a Jarrell-
been experimentally observed. Ash 0.25 mm monochromator. Low-density excitation was
employed to reduce the probability of any kind of nonlinear
The aim of this work is to correlate the MEH-PPV optical effects. Films (1 × 1 cm) were inserted between two
photoluminescence properties at several temperatures quartz windows held in an optical support. The optical holder
with relaxation processes using some complementary within the cryo-system (APD Cryogenics) was positioned to
and independent techniques: dynamic mechanical ther- minimize the scattering of light from the excitation beam in a
mal analysis (DMTA), thermally stimulated current way to stay immobile.
(TSC), 13C NMR using dipolar chemical shift correlation The samples were maintained under a dynamic vacuum of
(DIPSHIFT), and fluorescence spectroscopy. Since sev- 10-4 Torr during the measurements. Temperature was changed
eral spectral changes occur simultaneously with the from 40 to 400 K in steps of 10 K by a digital temperature
polymer relaxation processes, a kinetic model involving controller (Scientific Instruments model 9650) and allowed to
attain equilibrium for 5 min between each measurement. One
the dissociation of interchains to re-form intrachain spectrum was recorded at each temperature, and because all
excitons is proposed, attempting to explain the profiles of the experimental conditions were maintained constant, the
of the photoluminescence spectra at higher tempera- emission intensities were comparable over the entire experi-
One possible limitation of fluorescence spectroscopy A dynamic mechanical thermal analysis DMA 242-Netzsch
is its lack of ability to assign the secondary relaxation Thermisch Analyse equipment was used to perform the
thermal analyses. The dynamic mechanical characterization
processes to precise segments or groups of the polymer (DMA) was performed in the tension mode, under a steady
chain. To overcome this problem, we employed one- load of 1.78 MPa and a dynamic stress of 1.98 MPa, under a
dimensional 1D-DIPSHIFT NMR. That is a dipolar nitrogen flow of 50 mL/min. The scans were made over the
chemical shift correlation method, where the correlation temperature interval of 170-420 K at a heating rate of 2
between the dipolar and chemical shift interactions is K/min at frequencies of 1, 5, 10, 16, 20, 25, and 33 Hz. Each
used to provide information about molecular reorienta- sample was cut from chloroform cast films to a small rectan-
tions associated with relaxations in solid materi- gular sample, 10 mm long, 4.5-5.2 mm wide, and about 0.02
als.27,29,30 Regarding the time scale, DIPSHIFT experi- mm thick.
ments are most sensitive to motions occurring with rates The activation energy was calculated by plotting the fre-
quency f vs T-1 for the loss modulus (E′′) according to the
ranging from 1 to 30 kHz. Molecular motions occurring
Arrhenius law (eq 1):
at these rates scale down the anisotropic 13C-1H
magnetic dipolar coupling, which usually is of the order f ) f0 exp(-E/RT) (1)
Macromolecules, Vol. 38, No. 3, 2005 Relaxation Processes in MEH-PPV 927
where f is the frequency (Hz), f0 is the preexponential factor
(Hz), E is the activation energy (J mol-1), T is the absolute
temperature (K), and R is 8.32 J K-1 mol-1.
Nuclear magnetic resonance (NMR) experiments were per-
formed using a Varian Inova spectrometer at 13C and 1H
frequencies of 100.5 and 400.0 MHz, respectively. A Varian 7
mm MAS double-resonance probe head with variable temper-
ature (VT) was used. The spinning speed was controlled by a
Varian pneumatic system that ensures a rotation stability of
(2 Hz. Typical π/2 pulses lengths of 3.5 and 4.0 µs were
applied for 13C and 1H, respectively. A proton decoupling field
strength of 60 kHz, cross-polarization time of 1 ms, and recycle
delays varying between 3 and 5 s were used. The temperature
dependence of 13C-1H dipolar couplings were measured using
1D dipolar chemical shift correlation (1D-DIPSHIFT) experi-
ments.34,35 1H-1H homonuclear decoupling was achieved by
the frequency-switch-Lee-Goldburg (FSLG) pulse sequence
performed with phase modulation and a field strength of
approximately 80 kHz.34,35 The maximum evolution time in
the 1D-DIPSHIFT experiments was 191.5 µs, which corre-
sponds to a spinning frequency of 5222 Hz. The scaling factor
of the FSLG sequence was experimentally obtained using
alanine and glycine as reference samples, whose dipolar
coupling values for CH, CH2, and CH3 groups are 13.7, 16.3,
and 22.8 kHz, respectively.
Thermally stimulated current (TSC) experiments were Figure 1. Photoluminescence spectra at several temperatures
performed with samples in the form of square thin films (25 (from 40 to 400 K) for MEH-PPV spin-coated films: (a) spun
× 25 mm), 50 mm thick, covered on both sides with aluminum from chloroform; (b) spun from toluene. λexc ) 21 270 cm-1.
electrodes of about 20 cm in diameter, deposited by evapora-
tion. An Edwards cryogenic chamber and high-vacuum system tures, from 40 to 410 K, of spin-coated films of MEH-
was used in conjunction with a Gefran temperature controller, PPV from both toluene and chloroform solutions. Fluo-
model 3300. The electric current on depolarization was mea- rescence spectra at higher temperatures (T > 310 K)
sured by a Keithley model 617 electrometer. Temperature and are broader, centered at 16 950 cm-1, with a longer red-
current data were collected by a computer. The following steps edge tail. The blue-shifted peak can be assigned to
were performed in the measurements: (i) the temperature was
raised to 393 K, and a polarization electric field of 20 MV/m
intrachain excitons and the red-edge emission to inter-
was applied during 30 min; (ii) under the action of the electric chain species.5-10,13-17 Spectra at lower temperatures
field the sample was cooled to 77 K at 5 K/min; (iii) a short (T < 220 K), centered around 16 390 cm-1, were as-
circuit until a current of 10-15 A was registered; and (iv) the signed to interchain excitons of MEH-PPV, as previ-
temperature increase up to 450 K at rate of 5 K/min and the ously observed for concentrated solutions.5-8 No emis-
depolarization electric current values were registered as a sion around 14 285 cm-1 was found, indicating complete
function of temperature. The vacuum in the system was held absence of emitting excimers.39 In addition to the
at 10-7 Torr throughout the experiment. The activation energy temperature dependence of the spectral profile, there
was calculated using the method of Lei et al.38 The thermally
is also an increase in the emission intensity at the blue
stimulated current is expressed by
edge, which is in agreement with the expected higher
quantum yield of the intrachain excitons as compared
[ (kT) - D∫ exp(- kT′) dT′]
I ) C′ exp -
(2) to the interchain species.8-10,13-17
It has been observed that the spectral profile of
where C′ ) P0S/τ0 and D ) 1/hτ0; T is the absolute tempera- MEH-PPV varies with temperature and with the
ture, k the Boltzmann constant, and A the activation energy solvent used to spin the polymer solution, demonstrat-
corresponding to a determined relaxation process. C′ and D ing a memory effect from the conformation in solution
are coefficients independent of T and A. With some math-
ematical manipulation one gets
even after annealing the samples. The narrower spectra
found for films spun from toluene are compatible with
(n + 1)! a more ordered material, while a broader distribution
C ) a1 + ∑(1 - a
a3n(-1)n (3) of conformations is found for films spun from chloro-
form.8-10,13-17 The full width at half-maximum (fwhm)
(Figure 2a) is a parameter that can describe both the
where a2 ) Ti/Tp, a3 ≡ (Tp - Ti)/Ti; Tp is the temperature heterogeneity of the microenvironment around the
corresponding to the relaxation and Ti the lower temperature fluorophore and the spectral overlap resulting from the
immediately closer to Tp; t0 is the relaxation time, h is the presence of different intrachain conformations.40 Both
heating rate, S is the electrode area, and P0 is the initial
effects are effectively present in MEH-PPV films,
Using eq 3, C can be numerically determined and the broadening the emission band. Additionally, the pho-
activation energy is estimated according to toluminescence spectrum is further broadened by the
presence of interchain species. Consequently, the fwhm
kTpTi kTp2e-A/kTp values in the range of 1000-900 cm-1 are orders of
A)C and τ0 ) (4) magnitude larger than expected for homogeneous broad-
Tp - Ti hA
ening of species with decays on the pico- to nanosecond
time scale. Therefore, the resulting spectral shape
Results and Discussion reflects the cooperative effects of homogeneous and
Photoluminescence Spectra. Figure 1 depicts the inhomogeneous broadening, conformational disorder,
photoluminescence (PL) spectra at several tempera- and multiple species decays.
928 Cossiello et al. Macromolecules, Vol. 38, No. 3, 2005
Figure 3. Kinetic scheme for the fluorescence decays of
MEH-PPV films, where M is the ground-state chromophore,
M* is an excited-state species, I is the intrachain exciton, D*
is the excited-state aggregate, knr and kr are the radiationless
and radiative rate constants, respectively, ka(S*LD) is the rate
constant for the intrachain exciton forming an excited dimer,
and kd(S*LD) is the rate constant for the aggregated dissocia-
tion re-forming the intrachain exciton.
continuous spectral shift being observed from 300 to 400
K (Figure 2b).
The dependence of the integrated and normalized
photoluminescence intensities on temperature is shown
in Figure 2c. Each intensity value was taken as the ratio
between the integrated fluorescence (area under the
entire spectrum plotted in wavenumbers) at a given
temperature and the integrated intensity at the lowest
measured temperature, IF(T)/IF(T0). We have considered
IF(T0) as the value measured at 40 K, although rigor-
ously IF(T0) should be at 0 K. Taking into account that
the emission intensity is almost temperature indepen-
dent below 140 K, we can assume that those radiation-
Figure 2. (a) Fwhm, (b) photoluminescence peak maxima less processes strongly dependent on temperature are
(cm-1), and (c) integrated and normalized intensity, IF(T)/IF- inhibited below this temperature.8,18
(T0), at several temperatures for MEH-PPV films: spun from Two isoemissive points were found for both samples,
toluene (0) or spun from chloroform (9). λexc ) 21 270 cm-1. around 16 714 and 16 605 cm-1, suggesting that some
kind of thermal equilibrium involving two different
There are some hypotheses postulated to explain the species might be operating. Assuming different species
blue shift of the photoluminescence spectra at higher emitting with distinct efficiencies from 30 up to 410 K,
we could explain the simultaneous blue shift and higher
temperatures (Figures 1 and 2b). Assuming that only
intensity upon heating, considering the kinetic scheme
intrachain excitons are responsible for the photolumi-
depicted in Figure 3, where the dissociation of some
nescence, the blue shift can be attributed to (i) thermally
interchain species gives rise to an intrachain exciton.
induced torsional motions shortening the conjugation
According to this scheme, and in absence of excimeric
lengths and (ii) differences in the Huang-Rhys coupling species, some short chains can be vibronically excited
factors (S) for chains with distinct conjugation lengths, (SS*) and rapidly relax to longer intrachain electroni-
leading to differences in the relative intensities of the cally excited states (SL*) through vibrational relaxation
zero- and higher-order phonons, producing changes in and internal conversion (kS). This SL* species can decay
the spectral profile.17,26 Although these possibilities nonradiatively to an interchain trap producing an
explain the blue shifts at higher temperatures, these interchain exciton (D*) (ka(SL*D)) or can decay to an
properties cannot explain the blue shift and intensity interchain excimer (E*) (ka(SL*E)). This last pathway
enhancements for increasing temperatures. To explain was ruled out because excimer emission at 700 nm was
the simultaneous change of the peak position and not observed. On the other hand, this longer intrachain
emission intensity, we have assumed that different species (SL*) can decay radiatively (kr(SL)) or nonradia-
species are emitting in each temperature range, in tively (knr(SL)). When the excited intrachain segments
agreement with data reported for PPV.17,26 The emission undergo faster radiative decay to the electronic ground
of isolated PPV chains at lower temperatures (10 K) is state, the observed emission is at hνF(L) ) 16 950 cm-1
red-shifted by at least 400 cm-1 as compared to that at (Figure 1). This is the most important emission at
higher temperatures (300 K).30 This effect cannot be temperatures above 320 K. The excited interchain
explained by simple thermal population of states, which species (D*) could also decay radiatively (kr(D*) or
is only 208 cm-1. The difference between the emission nonradiatively (knr(D*) (Figure 3). When the decay is
maxima at 300 and 40 K is 220 cm-1, which, in radiative (D* f D), the emission takes place at the red
principle, could be attributed to the thermal population edge of the intrachain excitons (hνF(D) ) 16 390-16 500
of states. However, the peak position is not a continuous cm-1) (Figure 1). This is the higher intensity emission
function of the temperature increment: from 40 to 200- occurring below 200 K and is responsible by the longer
220 K the peak position is essentially constant, with a red edge tail of the emission spectrum above this
Macromolecules, Vol. 38, No. 3, 2005 Relaxation Processes in MEH-PPV 929
Figure 4. Arrhenius plot for the interchain/intrachain inten-
sity ratio (I15385/I16950) vs 1/T for MEH-PPV films spun from
chloroform (9) and toluene (0). λem(D) ) 15 385 cm-1 and λem-
(SL) ) 16 950 cm-1.
temperature. Because of the higher relative quantum
yield of the intrachain relative to the interchain exci-
tons, the integrated intensity at higher temperatures
increases, even though the radiationless rates (such as
internal conversion, vibrational relaxation, and inter-
system crossing, knr(S,L,D)) also become more effi-
Therefore, we considered that the relative intensity Figure 5. DMTA plots for a film of MEH-PPV at several
changes at 16 950 and 16 390 cm-1 depend on the frequencies.
population of intrachain and interchain species, and for
T > 300 K the dissociation of interchain species becomes conjugated chain. Larger changes are attributed to
an efficient process. The temperature dependence for motions of longer segments. Thus, we assign the lower
interchain dissociation can be described by the ratio of temperature process, occurring at 210 ( 10 K, to a
the emission intensity at 16 950 cm-1 (where the intra- secondary process (β-relaxation) and the higher tem-
chain is preferentially emitting) and at 16 390 cm-1 perature process, at 330 ( 10 K, to the glass transition
(where we are assuming that only the interchain exciton (R-relaxation). The net result that can be obtained from
is contributing to the emission signal). We assume a the above discussion is that the glass transition and the
simplified kinetic model where chain segments form dissociation of aggregated emitting species are strongly
interchain species (D*) with a rate constant ka(S*LD) correlated events.
and undergo dissociation, re-forming intrachain exci- Dynamical Mechanical Thermal Analysis. To
tons, SL*, with a rate constant kd(S*D).8,18,26,41 This gain further insight into the role played by chain
kinetic scheme is similar to that developed for the mobility on the photophysical changes occurring at 330
temperature dependence of excimer emission.26 Accord- ( 10 and 210 ( 10 K, DMTA experiments were run from
ing to our experimental data, at higher temperatures 140 to 420 K (Figure 5). Both storage and loss moduli
(T > 320 K) the efficiency of the interchain D* emission showed two broad relaxation processes: at 340 and at
is lower than of the intrachain excitons, kd . kD (rate 220 K, which we previously assigned to the R- and
constants for the interchain deactivation include radia- β-relaxation processes, respectively. The relaxation tem-
tive and radiationless rates). At lower temperatures (T peratures were in the same range as those determined
< 200 K), ka(S*LD) . kd(S*D) and ka(S*LD) . kS(L) by fluorescence spectroscopy. The R-relaxation process
where kS(L) ) kr(SL) + knr(SL) is the rate constant for observed by DMTA was also consistent with that
the intrachain deactivation including radiative and previously determined by DSC, Tg ) 338 K. Arrhenius
radiationless rates, and the emission arises preferen- plots (Figure 6) with data from experiments run at
tially from the interchain excitons. Considering this as several frequencies gave the activation energy for each
a typical example of chemical equilibrium involving relaxation process as 85.4 and 29.1 kJ mol-1 K-1,
association and dissociation, the temperature depen- respectively, for Tg and β-relaxation processes, indicat-
dence of the intensity ratio IF(D*)/IF(SL*) can be repre- ing that the β-relaxation involves shorter segments of
sented as an Arrhenius plot (Figure 4), where the the polymer chain.
emission for D* and SL takes place at 15 380 and 16 950 Thermal Stimulated Current. In addition to the
cm-1, respectively. DMTA we have also measured the relaxation processes
All plots in Figure 2 displayed two distinct temper- by depolarization of thermal stimulated current using
ature ranges for the changes in spectral behavior: at samples which were polarized at 390 and 430 K. The
210 ( 10 K producing changes with smaller magnitudes depolarization currents were recorded (Figure 7), show-
and at 330 ( 10 K producing changes with greater ing two main relaxation processes: one at a lower
magnitudes, where interchain dissociation is taking temperature range, from 100 up to 240 K, and another
place. Usually, slope changes of fluorescence intensity at a higher temperature range, from 300 to 370 K. Both
can be attributed to changes in nonradiative rate sets of transitions were located at the same temperature
constants and in polymer systems to polymer relaxation ranges as those observed by DMTA and photolumines-
processes.9,10,13-15 Smaller changes may be assigned to cence, which were previously assigned to β-relaxation
motions of smaller groups or lateral segments noneffi- and glass transition. Each one of these transitions
ciently coupled with the polymer backbone or with the exhibited subcomponents associated with sequential
930 Cossiello et al. Macromolecules, Vol. 38, No. 3, 2005
Figure 6. Arrhenius plots for the β (a) and R (b) relaxations
by DMTA. Figure 8. MEH-PPV repetitive unit (a) and magic-angle-
spinning NMR spectra of MEH-PPV with the corresponding
line assignments at (b) 253 and (c) 323 K.
smaller magnitude of the spectral, TSC, and DMTA
13C NMR Analysis. The identification of the isotropic
chemical shift for each chemical group in the 13C CP/
MAS spectrum of MEH-PPV was achieved on the basis
of typical chemical shift values. The repetitive units and
typical 13C CP/MAS spectra of MEH-PPV at 253 and
323 K are shown in Figure 8. Cross-polarization experi-
ments with dipolar dephasing were also applied to
distinguish protonated from nonprotonated carbons.35
This helped in the identification of the main chain
Figure 7. TCS plots for a MEH-PPV spin-coated film carbon resonances, which appear with considerable
polarized at 390 (9) and 430 K (O).
superposition in the NMR spectra. Thus, the line at 126
ppm was attributed to phenylene carbons 1 and 4, while
movements of polar segments of the polymer, distinctly the line at 120 ppm was attributed to the CH vinylene
polarized by the electrical filed. The assignment of each groups (carbons 7 and 8). The lines at 11 and 23 ppm
subtransition requires further detailed experiments. were attributed to carbon 16 and 17 belonging to the
The calculated activation energies for the glass transi- ethyl side group, while the peaks at 14, 23, ∼29, 39,
tion and β-relaxation processes were 62.4 and 22.5 kJ and 72 ppm were ascribed respectively to carbons 15,
mol-1 K-1, respectively. The activation energy values (16 and 14), (13 and 12), 11, and 10, belonging to the
of the β-relaxation obtained by TSC and DMTA (29.1 hexyloxy side group. The resonance at 55 ppm is typical
kJ mol-1 K-1) are in very good agreement, whereas of methoxy groups, carbon 9. Finally, the lines at ∼106
those obtained for the glass transition differ of about and 151 ppm were identified as belonging to the CH
20 kJ mol-1 K-1 (85.4 kJ mol-1 K-1 for DMTA). This (carbons 2 and 5) and CO (carbons 3 and 6) phenylene
difference related to long-range motions is probably carbons, respectively.
associated with the mechanisms involved with the At 323 K the lines corresponding to the side-group
relaxation processes; i.e., DMTA involves the entire bulk carbons are narrower than at 253 K, showing an
while TSC involves movements of the polar groups of increase in side group mobility at the higher tempera-
the polymer chain. ture. Comparing the line corresponding to the side-
Although TSC, DMTA, and fluorescence spectroscopy group carbons at both temperatures, it was possible to
identified two relaxation processes in the same temper- observe different line widths, which relate to differences
ature ranged, only PL was able to demonstrate that the in rates of motion along the side chain. Specifically, on
higher temperature process involved interchain move- the basis of the line width for the peak attributed to
ments producing dissociation of the interchain complex. carbons 12 and 13 compared with carbons 14 and 16 in
On the other hand, no microscopic details can be the spectrum at 253 K, it is possible to conclude that
inferred for the β-relaxation, apart from the indication the mobility of the latter is faster than the former.
that it is correlated with the side groups, due to the Besides, the lines are broader for carbons nearer the
Macromolecules, Vol. 38, No. 3, 2005 Relaxation Processes in MEH-PPV 931
Figure 9. (a) Experimental and simulated DIPSHIFT curves for carbons 2, 5, and 9 vs temperature in MEH-PPV. The curves
are presented for a full rotor period with T2 effects included in the simulation. (b) Same as in (a) for carbons 10, 12, and 13. (c,
d) Normalized averaged dipolar couplings vs temperature for protonated carbons.
main chain, narrowing systematically for the carbons 0.33, suggesting that the CH3 side-group carbons ex-
closer to the end of the side group, indicating a slight periment extra dynamics associated with the bulk
mobility gradient along the side chains. motion of the side chain. This was confirmed by the
Molecular Motions in MEH-PPV Probed by behavior of the side-group CH carbons, where 〈υdip〉/υdip
DIPSHIFT Experiments. As mentioned, a study of decreases monotonically with temperature, showing the
MEH-PPV dynamics was carried out using 1D-DIP- increasing gain of mobility of this group as a function
SHIFT experiments. Simulation of the DIPSHIFT curves of temperature.
and corresponding fit of the experimental data provided Another interesting item to be pointed out is the
an estimation of the averaged dipolar coupling fre- temperature dependence of the DIPSHFT curves for
quency, 〈υdip〉. T2 effects, also considered in the simula- CH2 groups at different positions in the side chain.
tions, were responsible for the partial decay of the 1D- Because all the signals analyzed in this case are from
DIPSHIFT intensities at tr. CH2 groups, due to the temperature independence of
Figure 9 shows the temperature dependence of the the curve for carbon 10, it is advantageous to perform
averaged dipolar coupling frequency, normalized by the the normalization using the averaged CH coupling of
rigid limit value, 〈υdip〉/υdip, for several carbons along the this group, υC10. By doing so, the dynamic behavior
side chain. along the side chain was studied in comparison with
The 〈υdip〉/υdip curves vs temperature obtained for the dynamics of carbon 10. The temperature dependence
carbons 2, 5, and 9, as well as the rate 〈υdip〉/υdip ∼ 1 in
MEH-PPV, demonstrate the absence of molecular of the parameter 〈υdip〉/υC10 for all side chain CH2
motions in the polymer backbone on a kilohertz time groups is shown in Figure 9. The 〈υdip〉/υC10 tempera-
scale. Similar behavior was observed for the other ture dependences also have the same trend; i.e., while
protonated carbons in the main chain (not shown). it is constant for carbon 10 it decreases monotonically
Particular attention should be taken with the meth- with temperature for the other CH2 groups. Thus, these
oxy carbon, which presents 〈υdip〉/υdip ∼ 0.33, even results also point to an increasing mobility through the
though CH3 groups have the highest rigid lattice dipolar side chain with temperature.
coupling. This is typical for segments executing aniso- At this point it is worthwhile to compare the fre-
tropic motions, which partially average the correspond- quency scales to which experiments are sensitive. As
ing dipolar coupling. Actually, these experimental curves mentioned before, NMR experiments, such 1D-DIP-
are reproduced using a dipolar coupling of 7.6 kHz, SHIFT, are sensitive to motions occurring with rates
which is 3 times smaller than that expected for rigid ranging from 1 to 30 kHz, which are higher than the
CH3 groups (22.8 kHz), suggesting the presence of CH3 usual frequencies where DMTA experiments are per-
rotations around the C3 axis occurring at frequencies formed (hertz to few kilohertz). Then, because the rate
higher than 30 kHz. of the molecular motions is associated with temperature
Complementarily, a clear temperature dependence of and frequency, the same molecular relaxation in each
〈υdip〉/υdip was observed in the curves of side-group experiment will not necessarily appear at the same
carbons, as for example, carbons 14 and 16. This temperature. Similar time-correlated effects can be
demonstrated the presence of thermally activated mo- observed when comparing fluorescence spectroscopy and
lecular motions in the MEH-PPV side chain. For CH3 TSC (both involving reorientation of dipole moments)
side-group carbons, 〈υdip〉/υdip decays as a function of and NMR data. The major differences rely on the fact
temperature, and its value was always smaller than that DIPSHIFT NMR experiments measures CH bond
932 Cossiello et al. Macromolecules, Vol. 38, No. 3, 2005
reorientation, TSC measures the rate constants for (3) Samuel, D. W.; Rumbles, G.; Collison, C. J.; Friend, R. H.;
reorientation of the dipole moment after a prepolariza- Moretti, S. C.; Holmes, A. B. Synth. Met. 1997, 84, 497.
(4) Whitelegg, S. A.; Buckley, A.; Rahn, M. D.; Fox, A. M.;
tion, and fluorescence spectroscopy measures the tem- Bradley, D. D. C.; Palsson, L. O.; Samuel, I. D. W.; Webster,
perature dependence of a ratio among radiative and G. R.; Burn, P. L. Synth. Met. 2001, 119, 575.
nonradiative decays taking place on a nano- to picosec- (5) Sartori, S. S.; Feyter, S.; Hofkensn, J.; Auweraer, M. V.;
ond time scale. Schryver, F.; Brunner, K.; Hofstraat, J. W. Macromolecules
Thus, we cannot expect that the activation energy for 2002, 36, 500.
(6) Dogariu, A.; Vacar, D.; Heeger, A. J. Phys. Rev. B 1998, 58,
all of these processes should be similar, although, in 10518.
general, we observed a narrow temperature range where (7) Collison, C. J.; Wan, W. C.; Rothberg, L.; Hsich, B. R. J. Phys.
decay rates undergo some changes. When comparing Chem. A 1999, 103, 2394.
NMR with the time scale of PL measurements, the (8) Birks, B. Photophysics of Aromatic Molecules; Wiley: New
frequency range was always quite different if we (9) Klopffer, M.-H.; Bokobza, L.; Monnerie, L. Macromol. Symp.
consider a correlation with the radiative rate constants. 1997, 119, 119.
The PL time scale is from pico- to nanoseconds, faster (10) Luo, C.; Atvars, T. D. Z.; Meakin, P.; Hill, A. J.; Weiss, R. G.
than magnetic resonance. When compared with non- J. Am. Chem. Soc. 2003, 125, 11879.
radiative pathways, the time scale is even faster (from (11) Jakubiak, R.; Collison, C. J.; Wan, W. C.; Rothberg, L.; Hsich,
B. R. J. Phys. Chem. A 1999, 103, 2394.
pico- to sub-picoseconds). Nevertheless, what we observe (12) Lim, S.-H.; Bjorklund, T. G.; Gaab, K. M.; Bardeen, C. J. J.
in PL are relative changes of the rate constants, which Chem. Phys. 2002, 117, 454.
are produced by chain motions and which should take (13) Jenekhe, S. A.; Osaheni, J. A. Science 1994, 265, 765.
place on the same time scale as the NMR signals (14) De Deus, J. F.; Andrade, M. L.; Atvars, T. D. Z.; Akcelrud, L.
because they involve the same type of movements, Chem. Phys. 2003, 297, 177.
(15) Schurr, O.; Yamaki, S. B.; Wang, C.; Atvars, T. D. Z.; Weiss,
rotation of groups of the polymer chain. Thus, even R. G. Macromolecules 2003, 36, 3485.
though the detected relaxation temperatures in each (16) Vigil, M. R.; Bravo, J.; Baselga, J.; Atvars, T. D. Z. Curr. Org.
technique are in the same range, the activation energies Chem. 2003, 7, 197.
for the processes could be different due to the phenom- (17) Sheridan, A. K.; Lupton, J. M.; Samuel, I. D. W.; Bradley, D.
enological differences involved. D. Chem. Phys. Lett. 2000, 322, 51.
(18) Lakowicz, J. R. Principles of Fluorescence Spectroscopy;
Academic Press: New York, 1999; Chapter 4.
Conclusions (19) Gray, T.; Buenviaje, C.; Overney, R. M.; Jenekhe, S. A.; Zhen,
This work identified two relaxation processes in solid- L.; Jen, A. K. Y. Appl. Phys. Lett. 2003, 83, 2563.
(20) Bozano, L.; Tutle, S. E.; Carter, S. A.; Brock, P. J. Appl. Phys.
state MEH-PPV. DSC, DMTA, TSC, and fluorescence Lett. 1998, 73, 3911.
spectroscopy showed that the glass transition takes (21) Bozano, L.; Carter, S. A.; Scott, J. C.; Malliaras, G. C.; Brock,
place in the 330-340 K range. This is the temperature P. J. Appl. Phys. Lett. 1999, 74, 1132.
range where MEH-PPV is usually annealed and where (22) Lupton, J. M.; Samuel, I. D. W. Synth. Met. 2000, 111, 381.
there are remarkable changes of the morphology, such (23) Yu, J.; Hagashi, M.; Lin, S. H.; Liang, K. K.; Hsu, J. H.; Fann,
W. S.; Chao, C.-I.; Chuang, K.-R.; Chen, S.-A. Synth. Met.
as the surface roughness. In addition to the already 1996, 82, 159.
demonstrated morphological changes, we demonstrated (24) Hagler, A. T. W.; Pakbaz, K.; Voss, F. K.; Heeger, A. J. Phys.
by fluorescence spectroscopy that the glass transition Rev. B 1991, 44, 8652.
process involves dissociation of interchain species. We (25) Pichler, K.; Halliday, D. A.; Bradley, D. D.; Burn, P. L.;
Friend, R. H.; Holmes, A. B. J. Phys. Chem. Mater. 1993, 5,
also observed by DMTA, TSC, fluorescence spectroscopy, 7155.
and NMR that MEH-PPV undergoes a secondary (26) Rothberg, L. J.; Yan, M.; Papadimitrakopoulos, F.; Galvin,
relaxation process around 220 K that we called β-re- M. E.; Kwock, E. W. Synth. Met. 1996, 80, 41.
laxation. This is the temperature where some unex- (27) Munowitz, M. G.; Griffin, R. G.; Bodenhausen, G.; Huang,
plained behavior of several of the MEH-PPV electrical T. H. J. Am. Chem. Soc. 1981, 103, 2529.
(28) Lupton, J. M.; Samuel, I. D. W.; Monkman, A. P. Synth. Met.
and optical properties can be noted. Although TSC and 1999, 102, 1079.
fluorescence spectroscopy suggest that this is a very (29) Schaefer, J.; Stejskal, E. O.; Perchak, D.; Skolnick, J.; Yaris,
complex process involving the lateral substituents of the R. Macromolecules 1985, 18, 368.
backbone, only NMR unequivocally showed that the (30) Huster, D.; Xiao, L. S.; Hong, M. Biochemistry 2001, 40, 7662.
substituents are really involved. More specifically, CH2 (31) Bonagamba, T. J.; Becker-Guedes, F.; DeAzevedo, E. R.;
Schmidt-Rohr, K. J. Polym. Sci., Part B: Polym. Phys. 2001,
carbons 12-17 are the most important segments relax- 39, 2444.
ing in this temperature range, while groups directly (32) Becker-Guedes, F.; DeAzevedo, E. R.; Bonagamba, T. J.;
attached to the phenylene ring do not to contribute the Schmidt-Rohr, K. Appl. Magn. Reson., in press.
β-relaxation process. (33) Talhavini, M.; Atvars, T. D. Z. Quım. Nova 1995, 18, 298.
(34) Liu, Y.; Liu, M. S.; Li, X.-C.; Jen, A. K.-Y. Chem. Mater. 1998,
Acknowledgment. T.D.Z.A., R.F.C., A.C.B., E.R.d.A., (35) Opella, S. J.; Frey, M. H. J. Am. Chem. Soc. 1979, 101, 5854.
and T.J.B. thank FAPESP, CNPq, and MCT/PADCT/ (36) Vinogradov, E.; Madhu, P. K.; Vega, S. Chem. Phys. Lett.
IMMP for fellowships and financial support. L.A., 1999, 314, 443.
P.C.R., and A.C.B. thank CNPq and MCT/PADCT/ (37) Bielecki, A.; Kolbert, A. C.; Levitt, M. H. Chem. Phys. Lett.
IMMP for fellowships and financial support. We also 1989, 155, 341.
(38) Qing, Q. L.; Xuan, W.; Yong, F. J. Appl. Phys. 1992, 72, 4254.
acknowledge Prof. Carol Collins for useful discussions. (39) Chen, S.-H.; Su, A.-C.; Huang, Y.-F.; Su, C.-H.; Peng, G.-H.;
Chen, S.-A. Macromolecules 2002, 35, 4229.
References and Notes (40) Martins, T. D.; Yamaki, S. B.; Prado, E. A.; Atvars, T. D. Z.
J. Photochem. Photobiol. A: Chem. 2003, 153, 91.
(1) Akcelrud, L. Prog. Polym. Sci. 2003, 28, 875. (41) Pierola, I. F.; Horta, A. Rev. Iberamer. Polim. 1992, 1, 49.
(2) Nguyen, T.-Q.; Martini, I. B.; Liu, J.; Schwartz, B. J. J. Phys.
Chem. B 2000, 104, 237. MA048340I